J. Adhesion Sci. Technol., Vol. 20, No. 12, pp. 1357– 1365 (2006)
Also available online - www.brill.nl/jast
Effect of grafting of acrylic acid onto a PET ﬁlm surfaces
by UV irradiation on the adhesion of PSAs
YOUNG-WOOK SONG, HYUN-SUNG DO, HYO-SOOK JOO,
DONG-HYUK LIM, SUMIN KIM and HYUN-JOONG KIM ∗
Laboratory of Adhesion and Bio-Composites, Program in Environmental Materials Science,
Seoul National University, Seoul 151-921, South Korea
Received in ﬁnal form 3 July 2006
Abstract—To improve the peel strength between a pressure-sensitive adhesive (PSA) and its
substrate, grafting of acrylic acid (AA) onto the surface of poly(ethylene terephthalate) (PET) ﬁlm
was carried out. After AA was coated onto the surface of PET ﬁlms using a spin coater, the coated
PET ﬁlms were irradiated by UV. To investigate the surface chemistry and topography of the PET-
g-AA ﬁlms, the grafted surface of the PET ﬁlms was characterized by FT-IR spectroscopy, X-ray
photoelectron spectroscopy (XPS) and scanning probe microscopy (SPM). From these investigations,
the effects of grafting of AA at the surface of PET by UV irradiation were discussed. In addition,
to determine the effect of grafting on the adhesion between PSA polymer and PET-g-AA ﬁlms, peel
strength was measured after the PSA/PET-g-AA system was cured at various temperatures. As the
esteriﬁcation between PSA polymer and PET-g-AA ﬁlms occurred in the interfacial region, the peel
strength of the PSA/PET-g-AA system generally increased with increasing curing temperature.
Keywords: Pressure-sensitive adhesives (PSAs); grafting; acrylic acid (AA); PET; UV irradiation;
Surface modiﬁcation of polymers to improve their adhesion is being investigated
intensively. As the surface of a polymer generally shows a hydrophobic character,
improvement of physical properties of a polymer, including its adhesion, requires
modiﬁcation of the polymer surface. Therefore, methods for modifying the
surface characteristics of a polymer from hydrophobic to hydrophilic have received
signiﬁcant consideration. As the surface of a polymer is treated chemically
∗ Towhom correspondence should be addressed. Tel.: (82-2) 880-4784. Fax: (82-2) 873-2318.
1358 Y.-W. Song et al.
and/or physically, it becomes hydrophilic with consequent improvements in surface
physical properties of the polymer.
There are many useful treatment methods for the modiﬁcation of a polymer
surface such as treatment by plasma, electron beam radiation and UV-light-induced
grafting [1 –9]. Among these treatment methods for the surface modiﬁcation of
polymers, the photo-induced UV grafting onto polymer surfaces is a very interesting
method for obtaining desired properties for speciﬁc uses, because it allows the
surface characteristics to be altered without causing serious modiﬁcations to the
polymer bulk mechanical properties. In addition, UV grafting is an attractive way
to impart a variety of functional groups to a polymer [6 –9].
In this study, we used a poly(ethylene terephthalate) (PET) ﬁlm as a substrate.
Although a PET ﬁlm is very stable under UV irradiation, it is still efﬁcient enough
to induce grafting of vinyl monomer onto PET which is a potentially useful tool
for the chemical modiﬁcation of this polymer. In addition, a vinyl monomer is
covalently bonded to a site on the PET surface through grafting .
As the purpose of the UV-induced grafting is to improve the adhesion strength,
peel strength analysis is important in surface modiﬁcation study. Peel strength
represents the force required to peel away a tape from the substrate . Resistance
to peel is measured as the force required at a constant, pre-deﬁned, peel rate and
angle [10, 11].
2-Ethylhexyl acrylate (2-EHA, Junsei Chemical, Japan), vinyl acetate (VAc, Jun-
sei Chemical), methyl methacrylate (MMA, Junsei Chemical), glycidyl methacry-
late (GMA, Junsei Chemical), acrylic acid (AA, Junsei Chemical), ethyl acetate
(EAc, Samjun Chemical, South Korea, analytical grade) 2,2 -azobisisobutyronitrile
(AIBN, Daejung Chemicals & Metals, South Korea) and benzophenone (BP, Lan-
caster, UK) were used as received. PET ﬁlm of 25 µm thickness was supplied by
SK Chemical (South Korea).
2.2. Preparation of PSA
The PSA was prepared by solution polymerization as 40 wt% solids. The synthesis
method consisted in mixing 126 g 2-EHA, 10.5 g MMA, 1–3 g GMA, 10.5 g VAc,
0.3 g AIBN and 75 g EAc in a 500 ml, 4-neck ﬂask equipped with a stirrer, a
dropping funnel and a thermometer. The polymerization reaction was initiated at
70◦ C, and after this temperature was maintained for 30 min, a mixture of 150 g of
ethyl acetate and 0.6 g of AIBN was gradually added to the ﬂask over a duration of
2 h. The polymerization was subsequently carried out at 65 ± 5◦ C for another 4 h.
Improving the peel strength of PSAs by AA grafting on PET ﬁlm 1359
Scheme 1. Process of grafting of monomer (AA) onto PET by UV irradiation.
2.3. Grafting on PET ﬁlm
Grafting of AA onto the PET ﬁlm was carried out in a conveyer belt type, UV curing
machine equipped with a high-pressure mercury lamp (100 W/cm, main wavelength
340 nm) after the solution (90 wt% AA and 10 wt% BP) was coated onto the PET
ﬁlm using a spin coater (KPD-002, Kee-Bea, South Korea). The UV grafting times
were 0, 20, 40 and 60 s. To remove the ungrafted homopolymer and the ungrafted
AA, the cured ﬁlms were washed successively with toluene, methanol and water.
The modiﬁcation process of the PET ﬁlm with AA is shown in Scheme 1.
The surface modiﬁcation achieved was characterized using various analysis tech-
niques . Infrared spectroscopy is a very powerful tool for studying the chemical
structure in bulk materials as well as for providing molecular conformational details
which are inaccessible to most analytical methods . After grafting, the IR spec-
tra of PET-g-AA ﬁlms were obtained using an FT-IR ATR spectrometer (Nicolet
Magna 550 Series II, Midac, USA) with a resolution of 8 cm−1 . High-resolution,
three-dimensional images of the surfaces of the PET-g-AA ﬁlms were obtained by
a scanning probe microscope (SPM, Autoprobe CPTM , PSIA, USA) with a spring
constant k = 3.2 N/m in the non-contact mode. Statistical evaluation of the surface
topograhy was performed in a scanning area 5 × 5 µm2 . Surface chemistry was
characterized using X-ray photoelectron spectroscopy (XPS, ThermoVG, UK). The
spectrometer utilized a monochromatic Al Kα photon source operating at 15 kV and
15 mA. The software provided by the manufacturer was used for all XPS analyses.
2.5. PSA performance
The prepared PSA was coated onto the PET ﬁlm using a No. 18 K-bar, kept at room
temperature for 1 hr and then dried in an oven at 60◦ C for 20 min. After the dried
1360 Y.-W. Song et al.
PSA ﬁlms were applied onto PET-g-AA ﬁlms, they were placed in an oven at 25,
60, 100, 130 and 150◦ C for 10 min. Finally, PSA performance was evaluated in
terms of peel strength. Peel tests were conducted using a Texture Analyzer (TA-
XT2i, Stable Micro Systems, UK) at an angle of 180◦ with a crosshead speed of
3. RESULTS AND DISCUSSION
3.1. FT-IR analysis
FT-IR results on the PET-g-AA ﬁlm with various UV grafting times are shown in
Fig. 1. As only a small amount of AA was coated onto the surface of the PET-g-AA
ﬁlm by the spin coater, the spectra for the PET ﬁlms with various grafting times
were found to be close to those of the ungrafted PET ﬁlm.
Although it was difﬁcult to detect any changes in functional groups by the UV
grafting, some peaks due to AA were discernible. Indeed, there was an OH group
coming from AA, at 3430 cm−1 . To ﬁnd the effect of UV grafting, we calculated
the intensity ratio of the peak at 3430 cm−1 relative to that at 3050 cm−1 , which
is assigned to the aromatic C C in PET. The results are listed in Table 1.
As shown in Table 1, the peak intensity ratio of the OH group increased with
increasing UV grafting time. The ratio reached a maximum at the grafting time of 40
seconds, and then decreased, possibly due to the effect of AA homopolymerization.
These results conﬁrmed that the UV grafting effect of PET-g-AA was maximum at
Figure 1. FT-IR spectra of PET-g-AA ﬁlms with varying UV grafting time: (A) 0 s, (B) 20 s, (C) 40 s
and (D) 60 s.
Improving the peel strength of PSAs by AA grafting on PET ﬁlm 1361
3.2. XPS analysis
The results of surface chemical analysis of the PET-g-AA ﬁlms are presented in
Fig. 2 and Table 2. According to the results obtained by XPS in Fig. 2, the C1s
core-level spectrum was curve-ﬁtted with three peak components having binding
energies at 284.6, 286 and 288.5 eV, corresponding to the C C/C H, C O and
O C O functional groups, respectively [15 –17]. Also evident was the peak at
283.9 eV in the C1s spectra. This peak resulted from the inhomogeneous charging
effect on the polymer surface due to its insulating nature . As shown in Fig. 2,
the peak located at 284.6 eV, which was directly related to the nature of the polymer
(C C and C H), increased with increasing grafting time due to the grafting of AA
on the PET ﬁlms. On the other hand, the O1s peaks were decomposed into peaks
at 531.5 eV as hydroxide group ( OH), 532.8 eV as π -bonded oxygen (O C) and
533.3 eV as σ -bonded (O C) oxygen. These results were in agreement with the
OH peak intensity ratio of PET-g-AA ﬁlms with varying UV
UV grafting time (s) I3430 cm−1 /I3050 cm−1
Figure 2. C1s and O1s XPS spectra of the PET-g-AA ﬁlms with varying UV grafting time: (A) 0 s,
(B) 20 s and (C) 40 s.
1362 Y.-W. Song et al.
Atomic concentration (%) for the PET-g-AA ﬁlms as determined by
XPS for varying UV grafting time
UV grafting time (s) C1s O1s
0 71.8 28.2
20 71.8 28.2
40 75.5 24.5
reference values [19 –21]. Among the three peaks, the peak located at 533.3 eV,
which was assigned to σ -bonded (O C) oxygen, increased rapidly. This is further
evidence of AA grafting on the PET ﬁlm.
As listed in Table 2, it was found that the amount of carbon on the PET ﬁlm surface
increased, while that of the oxygen decreased as a result of the grafting process.
3.3. SPM analysis
There are certain characteristics in the topological analysis of a surface such as the
RMS roughness, average roughness and mean height. Generally, changes in the
surface roughness are quantiﬁed in terms of root-mean-square (RMS) value, given
as the standard deviation of the distribution of all height values within the surface
area of interest and is deﬁned as :
Rrms = z2 (x, y) dx dy,
Lx Ly 0 0
where Lx and Ly are the lengths of x-axis and y-axis, respectively. Although the
RMS surface roughness is a useful parameter for comparing surfaces, it is insuf-
ﬁcient to completely describe a surface and can lead to erroneous characterization
for surfaces possessing a variety of feature types. Therefore, in order to provide a
more meaningful description of the surface it is instructive to examine the complete
height histogram of the image. A height histogram of the image can also be used to
reconstruct height values and mean height, and thus it represents a superset of data
contained in an RMS surface roughness value .
As shown in Fig. 3, the surface roughness of the PET-g-AA ﬁlm increased
with increasing UV-grafting time. This result supports the hypothesis that surface
grafting can increase the surface roughness. In other words, the increasing surface
roughness signiﬁes occurrence of grafting reactions on the surface. However, the
surface roughness of the PET-g-AA ﬁlm decreased after the maximum grafting
at 40 s because of the decreased graft degree due to the removal of ungrafted
homopolymer and monomer. In general, homopolymer and ungrafted monomers
were removed by solvent such as methanol, acetone and toluene, at the condition of
excess UV irradiation times.
Improving the peel strength of PSAs by AA grafting on PET ﬁlm 1363
Figure 3. Surface roughness of the PET-g-AA ﬁlms with various UV grafting times.
Figure 4. Peel strength of PSA/PET-g-AA ﬁlms with various GMA contents as a function of curing
temperature. Numbers in the upper right hand corner refer to percentage of GMA.
3.4. Peel strength
Figure 4 shows the peel strength of the PSA/PET-g-AA ﬁlm systems with varying
GMA content. With increasing GMA content, the peel strength of PSA/PET-g-
AA increased because the hydroxide group of PSA reacts with the carboxylic acid
1364 Y.-W. Song et al.
Scheme 2. Mechanism of esteriﬁcation between PSA polymer and PET-g-AA.
group of PET-g-AA to produce esteriﬁcation. The mechanism, shown in Scheme 2,
consists of two steps. First, the epoxide ring of GMA is opened by the attack of the
hydroxide group in AA. Due to the esteriﬁcation occurring between GMA and AA,
the interface between the PSA polymer and PET-g-AA becomes stronger through
Although the peel strength of PSA/PET-g-AA increased with the increment of
GMA, the peel strength showed an irregular relationship with the increment of UV
curing temperature, as shown in Fig. 4. In fact, the peel experiments demonstrated
that the failure mode of PSA/PET-g-AA depended on the curing temperature. Since
the adhesion at the PSA/PET-g-AA interface was stronger than the cohesive strength
of the PSA, the failure mode of PSA/PET-g-AA was cohesive rather than interfacial.
However, one can see that the peel strength of PSA/PET-g-AA increased at about
150◦ C. It seems that the esteriﬁcation between PSA and PET-g-AA affected the peel
strength in spite of the cohesive failure of this system. These results conﬁrmed that
the peel strength of PSA/PET-g-AA increased with increasing GMA content due to
the process of esteriﬁcation.
In this study, we investigated the effects of UV grafting to improve the peel strength
of polymeric materials, such as PSAs. The use of AA as a vinyl monomer for
UV grafting altered the surface of the substrate (PET ﬁlm) from hydrophobic to
hydrophilic, as conﬁrmed by FT-IR, SPM and XPS analyses. With increasing
GMA content in the PSA, the peel strength of PSA/PET-g-AA increased, but a
cohesive failure occurred at curing temperatures above 130◦ C. The peel strength
results conﬁrmed the reaction mechanism for adhesion between PSA and PET-g-
AA. The mechanism consists of two steps. The ﬁrst step involves the scission of
the epoxy ring in GMA. The ring is opened by the attack of the OH group in AA.
The second step is the esteriﬁcation between the OH in GMA and the COOH in
AA. These two reactions increase the adhesion at the PSA/PET-g-AA ﬁlm interface.
The results of this study elucidated the effect of monomer grafting and explained
the increased adhesion strength observed between PSA and PET-g-AA.
Improving the peel strength of PSAs by AA grafting on PET ﬁlm 1365
This work was supported by the Brain Korea 21 Project.
1. R. Liepins, J. R. Surles, N. Morosoff and V. T. Stannett, J. Appl. Polym. Sci. 21, 2529 (1977).
2. Y. Avny, L. Rebenfeld and H. D. Weigmann, J. Appl. Polym. Sci. 22, 125 (1978).
3. P. D. Kale and H. T. Lokhande, J. Appl. Polym. Sci. 19, 461 (1975).
4. K. L. Mittal (Ed.), Polymer Surface Modiﬁcation: Relevance to Adhesion, Vol. 2. VSP, Utrecht
5. K. L. Mittal (Ed.), Polymer Surface Modiﬁcation: Relevance to Adhesion, Vol. 3. VSP, Utrecht
6. C. He and Z. Gu, Radiat. Phys. Chem. 68, 873 (2003).
7. A. Bhattacharya and B. N. Misra, Prog. Polym. Sci. 29, 767 (2004).
8. K. Kato, E. Uchida, E. T. Kang, Y. Uyama and Y. Ikada, Prog. Polym. Sci. 28, 209 (2003).
9. P. S. Curti, M. R. de Moura, W. Veiga, E. Radovanovic, A. F. Rubira and E. C. Muniz, Appl.
Surface Sci. 245, 223 (2005).
10. C. M. Chan, Polymer Surface Modiﬁcation and Characterization, Hanser Gardner, Cincinnati,
11. D.-J. Kim, H.-J. Kim and G.-H. Yoon, Int. J. Adhesion Adhesives 25, 288 (2005).
12. Y.-J. Park, H.-S. Joo, H.-J. Kim and Y.-K. Lee, Int. J. Adhesion Adhesives (2006) (in press).
13. I. Benedek, Pressure-Sensitive Adhesives and Applications. Marcel Dekker, New York, NY
14. Z. Zhu and M. J. Kelley, Polymer 46, 8883 (2005).
15. M. C. Zhang, E. T. Kang, K. G. Neoh and K. L. Tan, Colloids Surfaces A 176, 139 (2001).
16. E. Uchida, H. Iwata and Y. Ikada, Polymer 41, 3609 (2000).
17. E. Uchida, Y. Uyama, H. Iwata and Y. Ikada, J. Polym. Sci. A: Polym. Chem. 28, 2837 (1990).
18. S. Massey, D. Roy and A. Adnot, Nucl. Instrum. Methods Phys. Res. B 208, 236 (2003).
19. S. Jin and A. Atrens, Appl. Phys. A 42, 149 (1987).
20. L. T. Weng, C. Poleunis, P. Bertrand, V. Carlier, M. Sclavons, P. Franquinet and R. Legras,
J. Adhesion Sci. Technol. 9, 859 (1995).
21. M. Bou, J. M. Martin, Th. Le Mogne and L. Vovelle, Appl. Surface Sci. 47, 149 (1991).
22. P. Esena, C. Riccardi, S. Zanini, M. Tontini, G. Poletti and F. Orsini, Surface Coatings Technol.
200, 664 (2005).
23. W. Yoshida and Y. Cohen, J. Membr. Sci. 215, 249 (2003).